Symmetry and twins in the monophosphate tungsten bronze series (PO~2~)~4~(WO~3~)~2<i>m~</i> (2 {łeq} <i>m</i> {łeq} 14)
Pascal Roussel; Philippe Labbe; Daniel Groult; Acta Crystallographica Section B 56 (2000) 377–391; doi:10.1107/S0108768199016195

data_2102081
_publ_contact_author_address
;
Laboratoire CRISMAT-ISMRA 6 Bd Mal JUIN 14050 Caen, FRANCE
;
_publ_contact_author_email       pascal.roussel@ismra.fr
_publ_contact_author_fax         33231951600
_publ_contact_author_name        'Roussel Pascal'
_publ_contact_author_phone       33231452610
_publ_section_title
;
 Symmetry and twins in the monophosphate tungsten bronze series
 (PO~2~)~4~(WO~3~)~2<i>m~</i> (2 {\/leq} <i>m</i> {\/leq} 14)
;
_journal_date_accepted           1999-12-09
_journal_date_recd_electronic    1999-08-23
_journal_issue                   3
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              377
_journal_page_last               391
_journal_paper_category          FA
_journal_paper_doi               10.1107/S0108768199016195
_journal_volume                  56
_journal_year                    2000
_chemical_formula_sum            'O62 P4 W18'
_chemical_formula_weight         4425.1
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                90.00(2)
_cell_angle_beta                 90.20(2)
_cell_angle_gamma                89.78(2)
_cell_formula_units_Z            1
_cell_length_a                   5.2945(9)
_cell_length_b                   6.542(2)
_cell_length_c                   32.744(5)
_cell_measurement_reflns_used    17
_cell_measurement_temperature    293
_cell_measurement_theta_max      43
_cell_measurement_theta_min      5
_cell_volume                     1134.1(4)
_computing_cell_refinement       'SET4 (Enraf Nonius, 1989)'
_computing_data_collection       'CAD4 (Enraf Nonius, 1980)'
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Enraf Nonius CAD4'
_diffrn_measurement_method       'type 2'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     .71073
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       64
_diffrn_reflns_limit_l_min       -64
_diffrn_reflns_number            20410
_diffrn_reflns_theta_max         45
_diffrn_reflns_theta_min         2
_diffrn_standards_decay_%        <4
_diffrn_standards_interval_time  60
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    45.714
_exptl_absorpt_correction_T_max  .833
_exptl_absorpt_correction_T_min  .148
_exptl_absorpt_correction_type   gaussian
_exptl_crystal_colour            'dark blue'
_exptl_crystal_density_diffrn    6.477
_exptl_crystal_description       platelet
_exptl_crystal_F_000             1888
_exptl_crystal_size_max          158
_exptl_crystal_size_mid          144
_exptl_crystal_size_min          4
_refine_diff_density_max         1.443
_refine_diff_density_min         -1.340
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_all   2.79
_refine_ls_goodness_of_fit_obs   2.79
_refine_ls_number_parameters     200
_refine_ls_number_reflns         4661
_refine_ls_R_factor_all          .0572
_refine_ls_R_factor_gt           .0572
_refine_ls_shift/esd_max         .001
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/\s^2^(F)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_all         .0468
_refine_ls_wR_factor_ref         .0468
_reflns_number_observed          4661
_reflns_number_total             20041
_reflns_observed_criterion       I>3\s(I)
_cod_data_source_file            lc0016.cif
_cod_data_source_block           LC0016
_cod_depositor_comments
;
The following automatic conversions were performed:
'_exptl_absorpt_correction_type' value 'Gaussian' changed to 'gaussian'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 

The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Gaussian' changed to
'gaussian' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_cell_volume        1134.2(4)
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               2102081